Upload
others
View
2
Download
0
Embed Size (px)
Gradient correction scheme for bulk and defectpositron states in materials: New developments
Jan Kuriplach1 and Bernardo Barbiellini2
1Charles University, Prague, Czech Republic
2Northeastern University, Boston, MA, USA
13thInternational Workshop on Slow Positron Beam Techniques and Applications
September 15 - 20, 2013, Munich, Germany
Outline
1 Motivation
2 LDA and GGA for positrons
3 Computational methods
4 Results and discussions
5 Conclusions
Positron GGA SLOPOS-13, 2/28
Outline
1 Motivation
2 LDA and GGA for positrons
3 Computational methods
4 Results and discussions
5 Conclusions
Positron GGA SLOPOS-13, 2/28
Outline
1 Motivation
2 LDA and GGA for positrons
3 Computational methods
4 Results and discussions
5 Conclusions
Positron GGA SLOPOS-13, 2/28
Outline
1 Motivation
2 LDA and GGA for positrons
3 Computational methods
4 Results and discussions
5 Conclusions
Positron GGA SLOPOS-13, 2/28
Outline
1 Motivation
2 LDA and GGA for positrons
3 Computational methods
4 Results and discussions
5 Conclusions
Positron GGA SLOPOS-13, 2/28
Motivation
Outline
1 Motivation
2 LDA and GGA for positrons
3 Computational methods
4 Results and discussions
5 Conclusions
Positron GGA SLOPOS-13, 3/28
Motivation
In general
The positron lifetime (τ) and affinity (A+) are fundamental positroncharacteristics.
They are often used to interpret experimental data in positron defectstudies.
But even more importantly τ and A+ are properties which reflectfundamental interactions – electron-electron and electron-positron –in solids.
Comparing experimental and theoretical counterparts may teach usabout the validity of our theory, but it may also doubt aninterpretation of our experiment in some cases.
Studying electron-electron and electron-positron interactions is noteasy because all particles strongly interact.
But the efforts certainly pay off when a deeper understanding isachieved.
Positron GGA SLOPOS-13, 4/28
LDA & GGA
Outline
1 Motivation
2 LDA and GGA for positrons
3 Computational methods
4 Results and discussions
5 Conclusions
Positron GGA SLOPOS-13, 5/28
LDA & GGA
Basic ideas
The two-component density functional theory says that the groundstate total energy of a system composed of electrons and positrons(and nuclei) is a functional of the electron (ρ−) and positron (ρ+)density (E ≡ E[ρ−, ρ+]).
The local density approximation (LDA) means that theexchange-correlation part of the E[ρ−, ρ+] functional is constructedusing the quantities coming from theories of the homogeneouselectron gas.
In the case of generalized gradient approximation (GGA) thisexchange-correlation term depends also on the gradient of theelectron density (∇ρ−).
Positron GGA SLOPOS-13, 6/28
LDA & GGA
Enhancement details
In the GGA for electrons one can define a dimensionless parameter
ε =|∇ρ−|2
(ρ−qTF )2=
π|∇ρ−|2
4(ρ−)2(3π2ρ−)13
with 1/qTF being the local Thomas-Fermi screening length;
q2TF = 4(3π2ρ−)13 π .
Then, we postulate that the electron screening cloud around positronwithin GGA is reduced with respect to the LDA screening cloud by anexponential factor
∆ρ−GGA = ∆ρ−LDA exp (−αε)
where α > 0 is an empirical parameter to be determined bycomparison with experiment.
Positron GGA SLOPOS-13, 7/28
LDA & GGA
Enhancement details
Since the screening charge in LDA is in fact given by theenhancement factor (contact density) as γLDA − 1, we can define theGGA enhancement factor as follows
γGGA = 1 + (γLDA − 1) exp (−αε) .
In the original approach by Barbiellini et al. [PRB 51, 7341 (1995)],α = 0.22 using the LDA enhancement after Arponen and Pajanne:
γLDA = 1 + 1.23rs − 0.0742r2s + r3s/6 .
Recently, Boronski [Nukleonika 55, 9 (2010)] suggested to useperturbed hypernetted chain result [Stachowiak and Lach, PRB 48,9828 (1993)]
γLDA = 1 + 1.23rs − 0.1375r2s + r3s/6
with α = 0.10.
Positron GGA SLOPOS-13, 8/28
LDA & GGA
Enhancement details
Very recently Drummond et al. [PRL 107, 207402 (2011)] on thebasis of quantum Monte Carlo determined another LDA enhancementwhich reads
γLDA = 1 + 1.23rs − 3.38208r3/2s + 8.6957r2s −− 7.37037r7/3s + 1.75648r8/3s + 0.173694r3s .
In this case, we suggest to use α = 0.05 for the positron GGA.
For the purpose of testing, we also use the original enhancement ofBoronski and Nieminen [PRB 34, 3820 (1986)]
γLDA = 1 + 1.23rs + 0.8295r3/2s − 1.26r2s + 0.3286r5/2s + r3s/6 .
Positron GGA SLOPOS-13, 9/28
LDA & GGA
Positron treatment details
The positron ground state wave function is obtained by solving theSchrodinger equation[
−1
2∇2
r − V c(r) + V ep(r)
]ψ+(r) = E+ψ+(r) .
In the case of the positron correlation potential, the GGA is appliedas follows
V epGGA = V ep
LDA exp(−αε/3) .
The positron lifetime (τ) is calculated via the positron annihilationrate (λ) according to the formula
1
τ= λ = πr20c
∫dr ρ+(r) ρ−(r) γ[ρ−(r), ε(r)] =
∫dr λi(r) .
considering that ρ+ = |ψ+|2 .
The positron affinity is then determined as
A+ = µ− + µ+ .
Positron GGA SLOPOS-13, 10/28
Methods
Outline
1 Motivation
2 LDA and GGA for positrons
3 Computational methods
4 Results and discussions
5 Conclusions
Positron GGA SLOPOS-13, 11/28
Methods
Electronic structure
The WIEN2k code was used to obtain the electronic structure ofstudied systems.
An LDA approach used for electron-electron exchange-correlations.
This code is one of the most precise implementations of DFT forcrystalline systems.
The unit cell is divided into (non-overlapping) spheres centered atnuclei and an interstitial space.
The 3D electron density and Coulomb potential are calculated on theregular 3D mesh covering the unit cell.
∇ρ− is calculated numerically inside the unit cell (the 3D mesh forvalence electrons and radial mesh for core electron densities).
Numerical parameters (cutoff, potential and density expansions)checked carefully to warrant precise results (∼0.1 ps for lifetime).
Positron GGA SLOPOS-13, 12/28
Methods
Positron calculations
We use one of the variants of atomic superposition code to solve theSchrodinger equation for positrons using a real space method(conjugate gradient).
The 3D density and potential produced by the WIEN2k code are readinto the positron code.
The mesh spacing of the 3D mesh should be typically 0.10− 0.15 a.u.in order to get precise results.
I For defect calculations, we addadditional bulk cells at the sides ofthe defect supercell to avoidproblems with boundary conditions.
I The electron density and potentialare joined continuously at the facesof supercell.
Positron GGA SLOPOS-13, 13/28
Results
Outline
1 Motivation
2 LDA and GGA for positrons
3 Computational methods
4 Results and discussions
5 Conclusions
Positron GGA SLOPOS-13, 14/28
Results
Experimental considerations
In positron lifetime studies there is quite larger scatter among bulklifetime results obtained by different groups.
We used mostly experimental results from the review by CampilloRobles and Plazaola [Defect Diff. Forum 213-215, 141 (2003)] andadded also some newer measurements.
Differences at the level ∼10 ps are not rare (e.g. Al: 160–170 ps).
For example, McGuire and Keeble [J. Appl. Phys. 100, 103504(2006)] have shown that using three different wrap foil materials forthe source results in differences up to 6 ps in bulk lifetimes of Al, Ni,Zr, and Pb.
This complicates comparison with calculations and raises questionsabout the precision of lifetime measurements.
For defect studies, the situation is similar.
Positron GGA SLOPOS-13, 15/28
Results
Abbreviations
BN - Boronski and Nieminen [PRB 34, 3820 (1986)]
AP - Arponen and Pajanne [Ann. Phys. (N.Y.) 121, 343 (1979)]
GC - original GGA with AP and α = 0.22
SL - Stachowiak and Lach [PRB 48, 9828 (1993)]
SG - SL with α = 0.10 (after Boronski [Nukleonika 55, 9 (2010)])
DB - Drummond et al. [PRL 107, 207402 (2011)]
DG - DB with α = 0.05
We often use notation ’X+’ for the specification of experimentallifetimes’ range though it is not ideal.
Positron GGA SLOPOS-13, 16/28
Results
d-metal lifetimes (in ps)
Element BN AP GC SL SG DB DG Exp.
Fe 101 94 110 98 107 102 107 105+
Cu 106 98 120 103 114 107 113 110+
Zn 137 124 150 131 144 136 144 145+
Nb 121 111 123 116 123 121 124 120+
Ag 123 113 140 118 132 123 131 130+
W 100 92 103 97 102 101 103 105
Pt 96 89 105 93 101 97 101 99+
DG and SG give best agreement with experiment.GC is somewhat exaggerated.LDA approaches yield often too short lifetimes.
Positron GGA SLOPOS-13, 17/28
Results
d-metal affinities (in eV)
Element BN GC SG DB DG Exp.
Fe −4.31 −3.74 −4.03 −4.12 −3.98 −3.3
Cu −4.89 −4.20 −4.55 −4.68 −4.50 −4.3
Zn −5.34 −4.78 −5.07 −5.06 −4.91
Nb −3.99 −3.62 −3.81 −3.75 −3.65 −3.8
Ag −5.70 −4.96 −5.34 −5.45 −5.26
W −2.08 −1.70 −1.90 −1.90 −1.80 −1.9
Pt −3.95 −3.34 −3.66 −3.78 −3.62 −3.8
For affinities the situation is not that clear compared to lifetimes.There are not so many measurements.Resulting affinity values are influenced by the electron-electron
exchange-correlation approach considered.
Positron GGA SLOPOS-13, 18/28
Results
Alkali metal lifetimes (in ps)
Element BN AP GC SL SG DB DG Exp.
Li 300 259 283 277 295 304 316 291
Na 328 291 339 310 342 343 364 338
K 374 338 396 360 395 401 423 397
SG and GC give best agreement with experiment.DG lifetimes fall too long.There are doubts about the precision of original experiment
[Weisberg and Berko, Phys. Rev. 154, 249 (1967)].
Positron GGA SLOPOS-13, 19/28
Results
sp-metal lifetimes (in ps)
Element BN AP GC SL SG DB DG Exp.
Al 165 146 155 155 160 161 165 160+
Sn(β) 189 167 198 177 192 186 194 196+
Pb 189 167 202 177 194 187 196 200+
SG and DG give best agreement with experiment.BN, AP, and SL lifetimes usually too short.Less frequent measurements, data might not be always reliable.
Positron GGA SLOPOS-13, 20/28
Results
Group IV semiconductor lifetimes (in ps)
Element BN AP GC SL SG DB DG Exp.
C 93 87 102 91 98 95 99 98+
Si 211 186 222 197 214 208 217 216+
Ge 214 190 241 201 225 213 225 219+
Sn(α) 257 228 296 242 274 258 275 289
SG and DG give best agreement with experiment.BN, AP, and SL lifetimes usually too short.β-Sn sample could still contain some defects.
Positron GGA SLOPOS-13, 21/28
Results
Oxide lifetimes (in ps)
Oxide BN AP GC SL SG DB DG Exp.
MgO 118 109 145 114 132 119 128 130
Cu2O 147 134 177 141 162 147 158 156+
ZnO 144 132 183 138 162 145 157 151+
ZrO2 128 118 159 124 143 129 138 ∼140
SG and DG give best agreement with experiment.BN, AP, and SL lifetimes usually too short.Some experimental lifetimes uncertain.
Positron GGA SLOPOS-13, 22/28
Results
Positron GGA from the microscopic viewpoint
A comparison of Na (bcc) and Si (diamond) electron- andpositron-related quantities.
The comparison is done for a [100] line having two atoms at its ends.
DB and DG approaches are considered.
Gradient correction is important in the core region and for openstructures also at the interstitial space!!
Positron GGA SLOPOS-13, 23/28
Results
Positron GGA from the microscopic viewpoint
Positron GGA SLOPOS-13, 24/28
Results
Defect calculations
We have also examined non-relaxed single vacancies in Al, Si and Cu andcalculated lifetimes for them.
Element BN AP GC SL SG DB DG Exp.
Al 234 204 222 217 227 228 233 237–244
Si 242 211 254 225 245 239 249 270–273
Cu 163 147 184 155 174 159 169 180
Positron GGA SLOPOS-13, 25/28
Conclusions
Outline
1 Motivation
2 LDA and GGA for positrons
3 Computational methods
4 Results and discussions
5 Conclusions
Positron GGA SLOPOS-13, 26/28
Conclusions
Conclusions and outlook
We have calculated positron characteristics in selected, representativesolids based on reliable DFT electronic structure calculations.
Highly accurate electronic structures of studied materials wereconsidered.
Several LDA and GGA approaches were tested.
The SG and DG calculations seem to agree best with experimentallifetimes, except for alkali metals that would require new experimentaldata allowing for a more precise comparison.
Positron energetics (affinities) is also improved in new GGA schemesthough further studies are needed.
The original GGA scheme appears to overestimate the gradientcorrection.
Defect studies were also performed showing promising results, butrelaxations still need to be considered.
Positron GGA SLOPOS-13, 27/28
T h a n k y o u !
Support: Project OPEN-1-13 of the Czech National Supercomputing Center IT4Innovations
Discussions: Morten Eldrup, David Keeble, Ivan Prochazka
T h a n k y o u !
Support: Project OPEN-1-13 of the Czech National Supercomputing Center IT4Innovations
Discussions: Morten Eldrup, David Keeble, Ivan Prochazka
T h a n k y o u !
Support: Project OPEN-1-13 of the Czech National Supercomputing Center IT4Innovations
Discussions: Morten Eldrup, David Keeble, Ivan Prochazka